Different strategies of secondary phase incorporation into metallic sheets by friction stir processing in developing surface composites
© The Author(s). 2016
Received: 3 October 2016
Accepted: 5 November 2016
Published: 15 November 2016
Friction stir processing (FSP) is a solid-state processing method, which recently gained wide popularity to modify the microstructure of metallic surfaces and to produce surface composites. For the past decade, composites of different materials such as aluminum, copper, magnesium, titanium, and their alloys were successfully produced by FSP. The amount of secondary phase that is dispersed at the surface of the workpiece during FSP and the level of dispersion depend on many factors such as tool design, processing parameters, and type of material. Recently, the method of secondary phase incorporation into the surface metals was also considered as an important factor in developing surface composites by FSP. A few strategies such as groove filling, holes filling, sandwich method, direct method, and surface coating followed by FSP methods have been developed as promising ways of secondary phase incorporation into the surface of the materials during FSP. The aim of this review paper is to give a comprehensive summary of different methods developed to disperse the secondary phase into the surface of the workpiece during FSP to produce surface composites. The strategies have been explained, compared, and discussed to suggest an appropriate method based on the requirement to adopt in developing surface composites.
KeywordsFriction stir processing Surface composites Secondary phase Dispersing methods
Friction stir processing (FSP) is a solid phase processing technique, developed to alter the microstructure of metallic sheets without melting the material and by inducing intense plastic deformation with the help of a rotating non-consumable tool that contains a pin at the end (Mishra and Ma 2005). FSP has also been widely used to produce different metallic surface composites. Surface composites are a class of materials in which the surface contains dispersed secondary phase, and the core of the material remains the same. Centrifugal casting, chemical or physical vapor deposition, plasma spraying, and laser treatment are a few methods have been developed to produce surface composites (Kapranos et al. 2014; Nikhilesh and Krishan 2013; Ayers and Tucker 1980). All these techniques involve melting of the substrate except FSP in which material does not melt (Mishra and Ma 2005). Developing composites in solid state using FSP can address the issues associated with melting and solidification usually found in conventional processes. Aluminum, copper, titanium, magnesium, and their alloys are the mostly used metals as matrix materials and SiC (Mishra et al. 2003; Alidokht et al. 2013; Barmouz et al. 2011; Devaraju et al. 2013), WC (Khosravi et al. 2014), MoS2 (Alidokht et al. 2013), Al2O3 (Devaraju et al. 2013; Raaft et al. 2011; Yang et al. 2010; Sharifitabar et al. 2011; Devaraju et al. 2013; Azizieh et al. 2011; Faraji et al. 2011), CNTs (Liu et al. 2013; Morisada et al. 2007; Morisada et al. 2006), B4C (Madhusudhan Reddy et al. 2013; Sathiskumar et al. 2013a), Ni particles (Devinder and Bauri 2011), carbon fibers (Mertens et al. 2012), TiC (Sabbaghian et al. 2014), hydroxyapatite (Ratna Sunil et al. 2014a; Ratna Sunil, et al. 2014b; Farnoush, Sadeghi, et al. 2013; Farnoush, Bastami, et al. 2013), and graphite (Soleymani et al. 2012) are the widely used dispersing phases in producing surface composites using FSP.
Several studies have been carried out to estimate the potential of FSP to produce surfaces with enhanced surface hardness, wear resistance, and corrosion resistance and were clearly demonstrated in the literature (Faraji et al. 2011; Liu et al. 2013; Devinder and Bauri 2011; Ratna Sunil et al. 2014a; Ratna Sunil et al. 2014b; Soleymani et al. 2012; Mishra et al. 2014). The success of producing a composite using FSP depends on many factors such as tool design, processing parameters, and type of the material (Mishra et al. 2014). Recent studies have clearly shown the method of secondary phase introduction during FSP also influence the amount and level of secondary phase distribution at the surface (Gandra et al. 2011; Miranda et al. 2013). Therefore, the objective of the present review is to give a comprehensive summary of different methods developed to incorporate secondary phase into the surface of the material in developing composites using FSP with an emphasis given to compare and discuss the methods.
Composite fabrication by friction stir processing (FSP)
The stirring action of FSP tool can be used to incorporate and distribute secondary phase into the surface of a metallic sheet or plate, and a surface composite can be produced by FSP. As the FSPed region contains fine grains, after composites produced by FSP also exhibit fine grain structure (Mishra et al. 2014; Ratna Sunil et al. 2012; Ratna Sunil et al. 2014). Therefore, grain size reduction is another advantage along with incorporating the secondary phase particles in developing surface composites by FSP. Initially, Mishra et al. (2003) successfully demonstrated producing Al-SiC composite using FSP. Later, there are numerous studies carried out to develop different metal matrix composites using FSP. Usually, the secondary phase is in the form of particles filled in grooves or holes produced on the surface of the material, and then FSP is carried out to disperse the secondary phase into the matrix metal. These secondary phase particles are dispersed in solid state itself during FSP due to the material flow resulted from the plastic deformation of the matrix material. The level of distribution of these particles within the matrix depends on many processing parameters. The mechanism of material flow during FSP is clearly explained by Arbegast (Arbegast 2003; Arbegast 2008), which involves several independent deformation processes such as extrusion and forging along with simultaneous localized heating and cooling.
Different methods of secondary phase incorporation into the matrix by FSP
The way how the secondary phase is introduced into the matrix material is also one of most influencing factors that affects the successful fabrication of the composite using FSP besides many influencing parameters such as (i) tool geometry which includes shoulder diameter, pin profile, and dimensions; (ii) processing parameters such as tool travel speed, rotational speed, and load; and (iii) material type. There are different methods reported in the literature to incorporate the secondary phase into the matrix material during FSP, and every method has its own advantages and limitations.
Groove filling method
Holes filling method
Direct friction stir processing (DFSP) tool method
Surface coating followed by FSP method
Maximum thickness of surface composite layer achieved in different material systems using FSP and the corresponding method used to incorporate the secondary phase into the matrix
Method of secondary phase incorporation
Composite layer thickness (mm)
Wang et al. (2009)
Groove filling and closing
Shafiei-Zarghani et al. (2009)
Lim et al. (2009)
Yang et al. (2010)
SiC and MoS2
Alidokht et al. (2011)
Devinder and Bauri (2011)
Groove filling and closing
Sharifitabar et al. (2011)
Maxwell Rejil et al. (2012)
Graphite, Al2O3, and SiC
Anvari et al. (2013)
SiC and Al2O3
Surface coating and FSP
Miranda et al. (2013)
Surface coating and FSP
Mazaheri et al. (2014)
Groove filling and closing
Lee et al. (2006)
Morisada et al. (2006)
Groove filling and closing
Asadi et al. (2011)
Azizieh et al. (2011)
Faraji et al. (2011)
Mertens et al. (2012)
SiC and B4C
Holes filling and closing
Madhusudan Reddy et al. (2013)
Direct friction stir processing tool
Huang et al. (2014)
Ratna Sunil et al. (2014b)
Barmouz et al. (2011)
Groove filling and closing
Sarmadi et al. (2013)
Groove filling and closing
Sathiskumar et al. (2013b)
Holes filling and closing
Sabbaghian et al. (2014)
Akramifard et al. (2014)
Farnoush et al. (2013)
Farnoush et al. (2013)
Ghasemi-Kahrizsang and Kashani-Bozorg (2012)
Groove filling was the first method proposed in the literature to produce a composite by FSP (Mishra et al. 2003). It is simple and requires less machining. A straight groove can be produced on the workpiece using ordinary milling cutter. Recently, Gandra et al. (2011) has studied the position of the groove with respect to the tool pin and demonstrated that if the groove is placed under the pin, the powder distribution is found to be more compared with placing the groove outside the pin interaction area (advancing or retrieving). Another strategy was proposed by Heydarian et al. (2014) in groove filling method in which parallel grooves with gradient groove depths were produced and FSP was carried out. Compared with single groove, composite produced from the gradient grooves was found to have uniform distribution of the powder. Whereas the groove filling and closing method needs additional tools such as pin-less FSP tool, and also the process involves two cycles; one to close the groove, and the second to produce the composite. The amount of secondary phase that can be introduced into the workpiece is more in groove filling and closing method compared with simple groove filling method because it prevents the escape of filled particles during FSP.
Holes filling method gives possibility to introduce more quantity of powder compared with that of groove filling method. Escape of the powder during FSP is less in holes filling method compared with that of groove filling method. Similarly, holes filling and closing method gives more control over the particle incorporation compared with that of groove filling and holes filling methods but requires more operations. For applications, where more quantity is not necessary but slight modification is enough to alter the surface properties, simple groove filling method or groove filling and closing method can be adapted. Groove filling method is also appropriate to obtain thick composite layers compared with other processes as shown in Table 1. Of course, the thickness of a composite layer depends on the FSP tool pin dimensions and processing parameters. Where applications demand more amount of secondary phase at the surface, holes filling or holes filling and closing method can be chosen.
Compared with these groove filling and hole filling methods, sandwich method does not require any machining process before FSP. Also, it reduces the necessity of using additional tool (without pin) to close the groove or holes before FSP. As reported by Faraji et al. (2011) the distribution of secondary phase is uniform in sandwich method. But making the secondary phase into the form of layers or laminas is difficult particularly with hard and brittle ceramic materials. Also, the secondary phase may present in the matrix in the form of large particles after FSP as there is no control over the breakdown of the layers during the process. There are a few studies clearly demonstrated that if the dispersing particle size is reduced, the surface properties were found to be improved (Liu et al. 2013; Morisada et al. 2007; Sabbaghian et al. 2014; Ratna Sunil et al. 2014a; Ratna Sunil et al. 2014b; Miranda et al. 2013). Therefore, in sandwich method, control over the size of secondary phase particle resulted from the FSP within the matrix is very poor and completely depends on the processing parameters and the design of the tool.
Another interesting development in the method of particle incorporation during FSP is application of direct friction stir processing (DFSP) tool as proposed by Huang et al. (2014). Initial machining processes such as producing grooves or holes to fill the secondary phase particles on the surface of the workpiece or need of another pin-less tool to close the groove or holes can be completely eliminated by using DFSP tool which is an advantage. This approach in tool design introduces the secondary phase particles into the surface effectively. However, the penetration depth (thickness) is the main limitation in DFSP method. The thickness of surface composite layer produced by DFSP is relatively less compared with the surface composite produced by FSP, and tool fabrication is also complex. But the level of uniformity in the distribution of the secondary phase is superior compared with other methods. Overall, this tool design showed interesting results in developing surface composites by FSP, and in future, this design may be used to develop wide variety of metallic surface composites. Providing surface coating on the workpiece by different means before FSP has also shown promising results in successfully developing the surface composites. More amount of secondary phase can be introduced into the surface, but the thickness of the produced composite layer is less compared with the composites produced by the other methods. Similar to DFSP tool method, surface coating followed by FSP method gives the modified surface depth limited to a few hundreds of micrometers from the surface. Also, pre-coating requires additional processing which increases the overall work to produce a composite.
Based on the required thickness and the amount of secondary phase that is required to be dispersed at the surface of the workpiece, appropriate method can be chosen in developing surface composites using FSP. Among all of the methods proposed in the literature, one common limitation is producing composites with tailored composition. The composition of the composites produced by FSP can be approximately assessed by assuming that the dispersion is uniform. However, exact amount of secondary phase that is distributed in the matrix material is not the same throughout the processed region. Variation in the distribution of secondary phase also influences the material properties if not macroscopic but microscopic level. Majority of the work is being carried out on developing different composite systems, but focus on developing strategies to address these issues is inferior. Developing new strategies to increase the level of incorporation, distribution of secondary phase, and increasing the thickness of the affected surface layer is in a great need to utilize the high potential of FSP technique in producing surface composites. For example, Asadi et al. (2010) studied the effect of penetration depth (PD) of FSP tool and demonstrated that the PD also has a great influence on composite formation. Further, the authors have shown the effect of (PD) on composite formation again depends on tool travel and rotational speeds. But, the composite layer thickness was not clearly reported. Investigating the combined effect of method of particles incorporation, process parameters, and type of tool on successful fabrication of surface composites by FSP also enhance the knowledge to address challenges involved in this area. Composite fabrication using FSP has wide industrial applications, and also the process does not require huge capital investments. Existing computer numerical control (CNC) machines can be modified with appropriate attachments and FSP can be carried out. Therefore, industries can easily and rapidly adopt the process.
It has been well demonstrated that FSP has a great potential in developing metallic surface composites in solid state itself. Different methods were proposed to incorporate secondary phase particles into the surface of the workpiece during FSP. Groove filling, holes filling, sandwich, DFSP, and surface coating followed by FSP are the widely used methods to incorporate the secondary phase into the metallic surfaces using FSP. Groove filling or holes filling followed by closing groove or holes using flat shoulder (pin-less) tool prior to FSP has shown optimum method to disperse more amount of secondary phase. Other new methods such as sandwich method, direct FSP tool, and surface coating method also have shown interesting results. However, research on developing these strategies and need of new strategies to produce tailored composites is in a great need to make the FSP technique as a promising method for industrial applications.
The author declares that there is no conflict of interest directly or indirectly related to the present research work.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Akramifard, H. R., Shamanian, M., Sabbaghian, M., & Esmailzadeh, M. (2014). Microstructure and mechanical properties of Cu/SiC metal matrix composite fabricated via friction stir processing. Materials and Design, 54, 838–844.View ArticleGoogle Scholar
- Alidokht, S. A., Abdollah-zadeh, A., Soleymani, S., & Assadi, H. (2011). Microstructure and tribological performance of an aluminium alloy based hybrid composite produced by friction stir processing. Materials and Design, 32, 2727–2733.View ArticleGoogle Scholar
- Alidokht, S. A., Abdollah-zadeh, A., & Assadi, H. (2013). Effect of applied load on the dry sliding wear behavior and the subsurface deformation on hybrid metal matrix composite. Wear, 305, 291–298.View ArticleGoogle Scholar
- Anvari, S. R., Karimzadeh, F., & Enayati, M. H. (2013). A novel route for development of Al–Cr–O surface nano-composite by friction stir processing. Journal of Alloys and Compounds, 562, 48–55.View ArticleGoogle Scholar
- Arbegast, W. J. (2003). Modeling friction stir joining as a metal working process. In Z. Jin, A. Beaudoin, T. A. Bieler, & B. Radhakrishnan (Eds.), Hot deformation of aluminum alloys III. Warrendale: TMS.Google Scholar
- Arbegast, W. J. (2008). A flow-partitioned deformation zone model for defect formation during friction stir welding. Scripta Materialia, 58, 372–376.View ArticleGoogle Scholar
- Asadi, P., Faraji, G., & Besharati, M. K. (2010). Producing of AZ91/SiC composite by friction stir processing (FSP). International Journal of Advanced Manufacturing Technology, 51, 247–260.View ArticleGoogle Scholar
- Asadi, P., Besharati Givi, M. K., Abrinia, K., Taherishargh, M., & Salekrostam, R. (2011). Effects of SiC particle size and process parameters on the microstructure and hardness of AZ91/SiC composite layer fabricated by FSP. Journal of Materials Engineering and Performance, 20(9), 1554–1562.View ArticleGoogle Scholar
- Ayers, J. D., & Tucker, T. R. (1980). Particulate-TiC-hardened steel surfaces by laser melt injection. Thin Solid Films, 73(1), 201–207.View ArticleGoogle Scholar
- Azizieh, M., Kokabi, A. H., & Abachi, P. (2011). Effect of rotational speed and probe profile on microstructure and hardness of AZ31/Al2O3 nanocomposites fabricated by friction stir processing. Materials and Design, 32, 2034–2041.View ArticleGoogle Scholar
- Barmouz, M., Asadi, P., Besharati Givi, M. K., & Taherishargh, M. (2011). Investigation of mechanical properties of Cu/SiC composite fabricated by FSP: Effect of SiC particles size and volume fraction. Materials Science and Engineering A, 528, 1740–1749.View ArticleGoogle Scholar
- Devaraju, A., Kumar, A., Kumaraswamy, A., & Kotiveerachari, B. (2013). Influence of reinforcements (SiC and Al2O3) and rotational speed on wear and mechanical properties of aluminum alloy 6061-T6 based surface hybrid composites produced via friction stir processing. Materials and Design, 51, 331–341.View ArticleGoogle Scholar
- Devaraju, A., Kumar, A., & Kotiveerachari, B. (2013). Influence of addition of Grp/Al2O3p with SiCp on wear properties of aluminum alloy 6061-T6 hybrid composites via friction stir processing. Transactions of the Nonferrous Metals Society of China, 23, 1275–1280.View ArticleGoogle Scholar
- Devinder, Y., & Bauri, R. (2011). Processing, microstructure and mechanical properties of nickel particles embedded aluminium matrix composite. Materials Science and Engineering A, 528, 1326–1333.View ArticleGoogle Scholar
- Faraji, G., Dastani, O., & Akbari Mousavi, S. A. A. (2011). Effect of process parameters on microstructure and micro-hardness of AZ91/Al2O3 surface composite produced by FSP. Journal of Materials Engineering and Performance, 20, 1583–1590.View ArticleGoogle Scholar
- Farnoush, H., Sadeghi, A., Bastami, A. A., Moztarzadeh, F., & Mohandesi, J. A. (2013). An innovative fabrication of nano-HA coatings on Ti-CaP nanocomposite layer using a combination of friction stir processing and electrophoretic deposition. Ceramics International, 39, 1477–1483.View ArticleGoogle Scholar
- Farnoush, H., Bastami, A. A., Sadeghi, A., Mohandesi, J. A., & Moztarzadeh, F. (2013). Tribological and corrosion behavior of friction stir processed Ti-CaP nanocomposites in simulated body fluid solution. Journal of the Mechanical Behavior of Biomedical Materials, 20, 90–97.View ArticleGoogle Scholar
- Gandra, J., Miranda, R., Vilac, P., Velhinho, A., & Pamies Teixeira, J. (2011). Functionally graded materials produced by friction stir processing. Journal of Material Processing Technology, 211, 1659–1668.View ArticleGoogle Scholar
- Ghasemi-Kahrizsangi, A., & Kashani-Bozorg, S. F. (2012). Microstructure and mechanical properties of steel/TiC nano-composite surface layer produced by friction stir processing. Surface and Coating Technology, 209, 15–22.View ArticleGoogle Scholar
- Heydarian, A., Dehghani, K., & Slamkish, T. (2014). Optimizing powder distribution in production of surface nano-composite via friction stir processing. Metallurgical and Materials Transactions B, 45(b), 821–826.View ArticleGoogle Scholar
- Huang, Y., Wang, T., Guo, W., Wan, L., & Lv, S. (2014). Microstructure and surface mechanical property of AZ31 Mg/SiC surface composite fabricated by direct friction stir processing. Materials and Design, 59, 274–278.View ArticleGoogle Scholar
- Kapranos, C., Carney, A., & Jolly, P. M. (2014). Advanced casting methodologies: investment casting, centrifugal casting, squeeze casting, metal spinning, and batch casting. In H. Saleem (Ed.), Comprehensive materials processing (pp. 39–67). USA: Elsevier.View ArticleGoogle Scholar
- Khosravi, J., Beshrati Givi, M. K., Barmouz, M., & Rahi, A. (2014). Microstructural, mechanical, and thermophysical characterization of Cu/WC composite layers fabricated via friction stir processing. International Journal of Advanced Manufacturing Technology, 74(5–8), 1087–1096.View ArticleGoogle Scholar
- Kurt, A., Uygur, I., & Cete, E. (2011). Surface modification of aluminium by friction stir processing. Journal of Material Processing Technology, 211, 313–317.View ArticleGoogle Scholar
- Lee, C. J., Huang, J. C., & Hsieh, P. I. (2006). Mg based nano-composites fabricated by friction stir processing. Scripta Materialia, 54, 1415–1420.View ArticleGoogle Scholar
- Lim, D. K., Shibayanagi, T., & Gerlich, A. P. (2009). Synthesis of multi-walled CNT reinforced aluminium alloy composite via friction stir processing. Materials Science and Engineering A, 507, 194–199.View ArticleGoogle Scholar
- Liu, Q., Ke, L., Liu, F., Huang, C., & Xing, L. (2013). Microstructure and mechanical property of multi-walled carbon nanotubes reinforced aluminum matrix composites fabricated by friction stir processing. Materials & Design, 45, 343–348.View ArticleGoogle Scholar
- Madhusudhan Reddy, G., Sambasiva Rao, A., & Srinivasa Rao, K. (2013). Friction stir processing for enhancement of wear resistance of ZM21 magnesium alloy. Transactions of the Indian Institute of Metals, 66(1), 13–24.View ArticleGoogle Scholar
- Maxwell Rejil, C., Dinaharan, I., Vijay, S. J., & Murugan, N. (2012). Microstructure and sliding wear behavior of AA6360/(TiC + B4C) hybrid surface composite layer synthesized by friction stir processing on aluminum substrate. Materials Science and Engineering A, 552, 336–344.View ArticleGoogle Scholar
- Mazaheri, Y., Karimzadeh, F., & Enayati, M. H. (2014). Tribological Behavior of A356/Al2O3 Surface nanocomposite prepared by friction stir processing. Metallurgical and Materials Transactions A, 45(a), 2250–2259.View ArticleGoogle Scholar
- Mertens, A., Simar, A., Montrieux, H. M., Halleux, J., Delannay, F., & Lecomte-Beckers, J. (2012). Friction stir processing of magnesium matrix composites reinforced with carbon fibres: influence of the matrix characteristics and of the processing parameters on microstructural developments. In W. J. Poole & K. U. Kainer (Eds.), Proceedings of the 9th International Conference on Magnesium Alloys and their Apllications (pp. 845–850). Vancouver: http://hdl.handle.net/2268/120134. ISBN 850.
- Miranda, R. M., Santos, T. G., Gandra, J., Lopes, N., & Silva, R. J. C. (2013). Reinforcement strategies for producing functionally graded materials by friction stir processing in aluminium alloys. Journal of Material Processing Technology, 213, 1609–1615.View ArticleGoogle Scholar
- Mishra, R. S., & Ma, Z. Y. (2005). Friction stir welding and processing. Materials Science and Engineering Reports, 50, 1–78.View ArticleGoogle Scholar
- Mishra, R. S., Ma, Z. Y., & Charit, I. (2003). Friction stir processing: a novel technique for fabrication of surface composite. Materials Science and Engineering A, 341, 307–310.View ArticleGoogle Scholar
- Mishra, R. S., Partha Sarathi, D., & Kumar, N. (2014). Friction stir welding and processing. UK: Springer.View ArticleGoogle Scholar
- Morisada, Y., Fujii, H., Nagaoka, T., & Fukusumi, M. (2006). MWCNTs/AZ31 surface composites fabricated by friction stir processing. Materials Science and Engineering A, 419, 344–348.View ArticleGoogle Scholar
- Morisada, Y., Fujii, H., Nagaoka, T., Nogi, K., & Fukusumi, M. (2007). Fullerene/A5083 composites fabricated by material flow during friction stir processing. Composites: Part A, 38, 2097–2101.View ArticleGoogle Scholar
- Nikhilesh, C., & Krishan, K. C. (2013). Metal matrix composites (2nd ed.). New York: Springer.Google Scholar
- Raaft, M., Mahmoud, T. S., Zakaria, H. M., & Khalifa, T. A. (2011). Microstructural, mechanical and wear behavior of A390/graphite and A390/Al2O3 surface composites fabricated using FSP. Materials Science and Engineering A, 528, 5741–5746.View ArticleGoogle Scholar
- Ratna Sunil, B., Sampath Kumar, T. S., & Chakkingal, U. (2012). Bioactive grain refined magnesium by friction stir peocessing. Materials Science Forum, 710, 264–269.View ArticleGoogle Scholar
- Ratna Sunil, B., Sampath Kumar, T. S., Chakkingal, U., Nandakumar, V., & Doble, M. (2014a). Friction stir processing of magnesium–nanohydroxyapatite composites with controlled in vitro degradation behavior. Materials Science and Engineering C, 39, 315–324.View ArticleGoogle Scholar
- Ratna Sunil, B., Sampath Kumar, T. S., Chakkingal, U., Nandakumar, V., & Doble, M. (2014b). Nano-hydroxyapatite reinforced AZ31 magnesium alloy by friction stir processing: a solid state processing for biodegradable metal matrix composites. Journal of Materials Science: Materials in Medicine, 25, 975–988.Google Scholar
- Ratna Sunil, B., Sampath Kumar, T. S., & Chakkingal, U. (2014). Micro/nanofeaturing of biodegradable metallic implants: new opportunities. In B. B. Jha (Ed.), Proceedings of International Conference on Engineering Materials and Processes (pp. 50–54). Bhubaneswar: CSIR-Institute of Minerals and Materials Technology.Google Scholar
- Sabbaghian, M., Shamanian, M., Akramifard, H. R., & Esmailzadeh, M. (2014). Effect of friction stir processing on the microstructure and mechanical properties of Cu–TiC composite. Ceramics International, 40(8), 12969–123976.
- Sarmadi, H., Kokabi, A. H., & Seyed Reihani, S. M. (2013). Friction and wear performance of copper–graphite surface composites fabricated by friction stir processing (FSP). Wear, 304, 1–12.View ArticleGoogle Scholar
- Sathiskumar, R., Murugan, N., Dinaharan, I., & Vijay, S. J. (2013a). Effect of traverse speed on microstructure and microhardness of Cu/B4C surface composite produced by friction stir processing. Transactions of the Indian Institute of Metals, 66(4), 333–337.View ArticleGoogle Scholar
- Sathiskumar, R., Murugan, N., Dinaharan, I., & Vijay, S. J. (2013b). Role of friction stir processing parameters on microstructure and microhardness of boron carbide particulate reinforced copper surface composites. Sadhana-Acad P Eng S, 38(6), 1433–1450.View ArticleGoogle Scholar
- Shafiei-Zarghani, A., Kashani-Bozorg, S. F., & Zarei-Hanzaki, A. (2009). Microstructures and mechanical properties of Al/Al2O3 surface nano-composite layer produced by friction stir processing. Materials Science and Engineering A, 500, 84–91.View ArticleGoogle Scholar
- Sharifitabar, M., Sarani, A., Khorshahian, S., & Shafiee Afarani, M. (2011). Fabrication of 5052Al/Al2O3 nanoceramic particle reinforced composite via friction stir processing route. Materials and Design, 32, 4164–4172.View ArticleGoogle Scholar
- Soleymani, S., Abdollah-zadeh, A., & Alidokht, S. A. (2012). Microstructural and tribological properties of Al5083 based surface hybrid composite produced by friction stir processing. Wear, 278–279, 41–47.View ArticleGoogle Scholar
- Wang, W., Shi, Q.-y., Liu, P., Li, H.-k., & Li, T. (2009). A novel way to produce bulk SiCp reinforced aluminum metal matrix composites by friction stir processing. Journal of Material Processing Technology, 209, 2099–2103.View ArticleGoogle Scholar
- Yang, M., Xu, C., Wu, C., Lin, K., Chao, Y. J., & An, L. (2010). Fabrication of AA6061/Al2O3 nano ceramic particle reinforced composite coating by using friction stir processing. Journal of Materials Science, 45, 4431–4438.View ArticleGoogle Scholar